SECTION 5-04 HOT MIX ASPHALT (HMA) PAVEMENT
5-04.1 DESCRIPTION This work shall consist of providing and
placing one or more layers of plant-mixed hot mix asphalt
(HMA) on a prepared foundation or base in accordance with these
Specifications and the lines, grades, thicknesses, and typical
cross-sections shown on the Drawings.
HMA shall be composed of asphalt binder and Mineral Aggregate as
may be required, and then mixed in the proportions specified to
provide a homogeneous, stable, workable, and compactable
5-04.2 MATERIALS Materials shall meet the requirements of the
Bituminous Materials 9-02 Mineral Aggregates 9-03 Temporary
Pavement Marking 9-29.4
The grade of asphalt binder will be specified in the Contract
(also see Section 5-04.2(1)).
5-04.2(1) USE OF SUBSTITUTE MATERIALS The proposed use of
substitute or alternate materials by the Contractor in the
production of HMA
from those specified in the Contract shall be part of the
submittal as specified in Section 5-04.3(6) and shall require
approval of the Engineer.
Recycled asphalt pavement (RAP): Unless the Contract specifies
otherwise, the Contractor may propose the use of RAP (see Section
9-03.8(3)B). RAP shall not exceed 20% of the total weight of
aggregate in the HMA mix. RAP will not be allowed for asphalt
binders with grades of PG-70 or higher.
Grade of asphalt binder: Unless the Contract specifies
otherwise, the Contractor may propose the use of a substitute grade
of asphalt binder. The substitute grade of asphalt binder shall: 1.
meet the requirements of Section 9-02.1(4), 2. have a maximum
pavement design temperature that is equal to or greater than that
specified binder, and 3. have a minimum pavement design
temperature that is equal to or lower than that of the
specified binder. The Engineer approved substituted grade of
asphalt binder shall be used only in HMA of the same
class with the Contract-specified grade of asphalt binder.
Blending of asphalt binder, whether different manufacturers and/or
Suppliers and/or different grades, will not be permitted.
5-04.3 CONSTRUCTION REQUIREMENTS
5-04.3(1) TERMS RELATED TO HMA
In Sections 5-04, 9-02, 9-03.6, and 9-03.8, terms and phrases
used (such as design aggregate structure, nominal maximum aggregate
size, air voids, maximum aggregate size, binder content, etc.) and
abbreviations (such as JMF for job mix formula, Va, Ndesign, Gsb,
etc.) are consistent with and can be found in WSDOT Standard
Operating Procedure (SOP) 732 Volumetric Design for Hot-Mix Asphalt
(HMA) and such other documents that are incorporated by reference
within WSDOT SOP 732. WSDOT SOP 732, and other incorporated by
reference documents, are available in the current edition of the
Washington State Department of Transportations Materials Manual M
5-04.3(2) MIXING PLANT In addition to the requirements of
Section 1-06, the Contractor shall allow the Engineer safe
to stockpiles for sampling. An adequate and convenient space for
the Engineer to temporarily store and test samples shall be
Plants used for the preparation of HMA shall conform to the
following requirements: Equipment for Preparation of Asphalt
Binder: Tanks for the storage of asphalt binder shall be equipped
to heat and hold the binder at the required temperatures. The
heating shall be accomplished by steam coils, electricity, or other
approved means so that no flame shall be in contact with the
storage tank. The circulating system for the asphalt binder shall
be designed to ensure proper and continuous circulation during the
operating period. A valve for the purpose of sampling the binder
shall be placed in either the storage tank or in the supply line to
the mixer. Also see Section 5-04.3(5) for heating asphalt binder
Thermometric Equipment: An armored thermometer, capable of
detecting temperature ranges expected in the HMA mix, shall be
fixed in the asphalt feed line at a location near the charging
valve at the mixer unit. The thermometer location shall be
convenient and safe for observation by the Engineer.
The plant shall also be equipped with an approved dial-scale
thermometer, a mercury actuated thermometer, an electric pyrometer,
or another approved thermometric instrument placed at the discharge
chute of the drier to automatically register or indicate the
temperature of the heated aggregates. This device shall be in full
view of the plant operator and shall be convenient to observation
by the Engineer. Sampling and Testing of Mineral Aggregates: The
HMA plant shall be equipped with a mechanical sampler for the
sampling of the Mineral Aggregates by the Engineer (see Sections
1-06.1 and 1-06.2).
5-04.3(3) PAVING AND RELATED EQUIPMENT
5-04.3(3)A HAULING EQUIPMENT Trucks used for hauling HMA shall
have tight, clean, smooth metal beds. A cover fabricated of
canvas or other suitable material and of sufficient size to
completely protect the mixture from adverse weather shall be
securely attached to the truck. Whenever the weather conditions
during the workshift include, or are forecast to include,
precipitation or an air temperature less than 45 F, the cover shall
be securely attached to protect the HMA.
In order to prevent the HMA mixture from adhering to the hauling
Equipment, truck beds shall be sprayed with an environmentally
benign release agent. Excess release agent shall be drained prior
to filling with HMA. For hopper trucks, the conveyer shall be in
operation during the process of applying the release agent.
5-04.3(3)B PAVING EQUIPMENT
5-04.3(3)B1 GENERAL As specified in Section 1-05.9, the
Contractor shall replace Equipment producing defective work. When
requested by the Engineer, the Contractor shall be prepared to
timely provide HMA and
related Equipment manufacturers written operating instructions
and maintenance manual.
5-04.3(3)B2 HMA PAVERS HMA pavers shall be self-contained,
power-propelled units, provided with an internally-heated
vibratory screed or strike-off assembly and shall be capable of
spreading and finishing courses of HMA plant mix material in lane
widths specified on the Drawings.
The screed or strike-off assembly shall effectively produce a
finished surface of the required evenness and texture without
tearing, shoving, segregating, or gouging the HMA. Extensions will
be allowed provided they produce the same results, including ride,
density, and surface texture as obtained by the primary screed or
strike off assembly. Extensions without augers, vibration, and
heated screeds, shall not be used in the traveled way.
The paver shall be equipped with automatic screed controls with
sensors for either or both sides of the paver. The controls shall
be capable of sensing grade from an outside reference line, sensing
the transverse slope of the screed, and providing automatic signals
that operate the screed to maintain the desired grade and
transverse slope. The sensor(s) shall be constructed so it operates
from a reference line or a mat referencing device.
The Contractor shall furnish and install all pins, brackets,
tensioning devices, wire, and accessories necessary for
satisfactory operation of the automatic control Equipment. The
Contractor shall be prepared to provide samples of the above items
prior to installation when requested by the Engineer.
The transverse slope controller shall be capable of maintaining
the screed at the desired slope within plus or minus 0.1 percent.
The paver shall be equipped with automatic feeder controls,
properly adjusted to maintain a uniform depth of material ahead of
Pavers operating with an MTV shall have additional capacity as
specified in Section 5-04.3(3)B3.
5-04.3(3)B3 MATERIAL TRANSFER VEHICLES (MTV) An MTV shall be an
independent, self-powered device configured for transferring HMA
Equipment to the paver. An MTV shall also have the following
characteristics: Delivery System: The MTV shall have a high
capacity truck unloading system that receives HMA from the hauling
Equipment. The truck unloading systems shall be capable of
unloading a truck at a rate greater than the rate of placement by
Surge Capacity: The MTV shall be equipped with an integral
storage bin capable of holding 25 tons of HMA. In addition, the HMA
paver operating with an MTV shall be equipped with a hopper insert
that shall be able to contain 15 additional tons of HMA. Remixing
Equipment: The MTV shall be designed to provide HMA remixing prior
to discharging to the paver. Discharge Conveyor: The MTV shall be
equipped with a discharge conveyor that shall have the ability to
swivel so the MTV may be operated from an adjacent lane while
delivering HMA to the paver.
5-04.3(3)C ROLLERS Rollers shall be of the steel wheel,
vibratory or pneumatic tire type, in good condition and capable
of reversing without backlash. Operation of the roller shall be
in accordance with the manufacturers recommendations. The number
and weight of rollers shall be sufficient to compact the mixture in
compliance with the requirements of Section 5-04.3(9). The use of
Equipment that results in crushing of the aggregate will not be
permitted. Rollers producing pickup, washboard, uneven compaction
of the surface, displacement of the mixture, or other defective
work (see Section 1-05.7) will be rejected by the Engineer in
accordance with Section 1-05.9.
5-04.3(3)D PLANING BITUMINOUS PAVEMENT AND REQUIRED PRE-PLANING
5-04.3(3)D1 GENERAL Prior to planing, the Contractor shall meet
with the Engineer to discuss the planing operations as
specified in Section 5-04.3(17).
5-04.3(3)D2 PLANING BITUMINOUS PAVEMENT Planing bituminous
pavement shall be by the cold planing method only. Equipment shall
be of a
type that has operated successfully on work comparable to that
in the Contract and shall be subject to the Engineers approval
prior to use. Equipment shall be maintained in good working
condition while in use.
Cold planers shall be milling type Equipment capable of cutting
at least a 5 foot chord to a depth of up to four (4) inches in one
pass. For Contract or Engineer required planing depths in excess of
four inches and as the total depth requires, the first pass and all
succeeding passes shall each be to a maximum four inch depth, with
the final pass depth being four or fewer inches to achieve the
total depth. Smaller planers may be used for cutting around
castings and other metal objects to remain, and for making taper
cuts for butt joints.
Where metal is not visible on the surface but is detected below
the surface, the Contractor shall employ methods of pavement
removal that do not damage the detected metal if it is to remain,
and is beyond the 4 inch maximum depth of planing so as not to
damage Contractor Equipment. On areas where irregularities or
unavoidable obstacles make the use of mechanical planing Equipment
impractical, the planing shall be done with other Equipment or by
For mainline cold planing operations, the Equipment shall have
automatic controls with sensor for either or both sides of the
Equipment capable of sensing the proper grade from an outside
reference line. The automatic controls shall also be capable of
maintaining the desired transverse slope. The sensor shall be so
constructed that it operates from a reference line or multi-footed
ski-like arrangement. The transverse slope controller shall be
capable of maintaining the desired slope within plus or minus 0.1
5-04.3(3)D3 REQUIRED PRE-PLANING METAL DETECTION The Contractor
shall be aware that metal may be buried beneath the existing
Such metal may be rail track associated with Seattles former
street car system, or may be castings buried under asphalt overlay,
or other similar metallic items.
Before planing, the Contractor shall adequately sweep the entire
area of asphalt to be planed to detect buried metal.
If such metal is detected and is not indicated in the Contract,
the Contractor shall surface mark such detected metal and shall
notify the Engineer of such condition before planing as required by
Where the Drawings indicate the existence of metal not visible
on the existing pavement surface, the Contractor shall remove such
surface pavement material and verify the depth to metal before
planing. If the depth to metal is beyond the required depth of
planing, the Contractor shall note such and shall avoid planing
contact with such metal. If the depth to metal is within the depth
range of required planing, then one of two outcomes is required, as
1. If a metal casting, then the casting shall be treated as
specified in Section 7-20. 2. If a metal object other than a
casting, then the Engineer may require removal. If removal
is not addressed in the Contract, then this portion of work will
be addressed as extra work. Metal detection Equipment shall have
adequate sensitivity to detect metal hidden beneath existing
pavement surface to a depth of at least 4 inches. Where planing
is indicated to a depth greater than four inches, the Contractor
shall be prepared to make multiple planing passes with each pass
not exceeding the four inch depth. Before each planing pass of four
inch or less, the Contractor shall resweep the same area of asphalt
to detect metal.
Where the Engineer directs additional depth planing beyond that
required in the Contract, the Contractor shall again sweep for
metal before such additional depth planning, as described in this
Contractor planing Equipment damaged by metal buried within
asphalt shall be the sole responsibility of the Contractor.
5-04.3(4) PREPARATION OF STREET SURFACES
5-04.3(4)A PREPARATION CLASSIFICATION DESCRIPTIONS In preparing
surfaces, the following surface classifications apply: Treated
surfaces: cement concrete, asphalt concrete, brick, seal coat or
surface treatments. Untreated surfaces: crushed rock, gravel,
native subgrade, or oil mat surfaces. Bituminous surface treatments
are addressed in Section 5-02, and oil mat surfaces are
in Section 4-04. The work of preparing existing surfaces for
asphalt concrete or other bituminous Material overlay
shall be classified as follows: Surface preparation applies only
to treated surfaces, and Roadway preparation applies only to
5-04.3(4)B SURFACE PREPARATION TREATED SURFACES
5-04.3(4)B1 GENERAL When an existing treated surface is to be
used as a base for one or more courses of new asphalt
concrete, or other surfacing (see Sections 4-04 and 5-02), the
treated surface shall first be swept, cleaned, and patched as
1. Treated surfaces shall be swept with a power broom until free
from dirt and other foreign matter. Hand brooms shall be used to
clean omissions of the power broom. Fatty asphalt patches, grease
drippings and other objectionable Material shall be removed from
the existing pavement.
2. Excess asphalt joint filler shall be completely removed and
premolded joint filler shall be removed to at least 1/2-inch below
the surface of the existing pavement.
3. In order to obtain a sound base having uniform grade and
cross section, irregularities in the existing treated surface shall
be corrected prior to placement of the new asphalt concrete or
other bituminous surface treatment. Corrections shall be made by
planing, preleveling, grinding, patching or by placing new base
5-04.3(4)B2 PRELEVELING When a surface of the existing pavement
or old base is irregular, it shall be brought to a uniform
grade and cross section by preleveling. Existing surfaces not
requiring planing, but requiring other repair or requiring
preleveling, will be addressed in the Contract. If existing asphalt
overlay is planed and the surface to remain requires preleveling,
then the Engineer will direct preleveling before HMA wearing course
placement in accordance with Section 5-04.3(8). As soon as the
existing surface has been thoroughly cleaned, holes and
discontinuities in the surface and edges and edge breaks shall be
repaired as specified in the Contract. Patching shall be
accomplished prior to preleveling or installation of the first
asphalt course, whichever is applicable.
Preleveling Materials shall be the same HMA class of asphalt
concrete as the wearing course or an acceptable alternate approved
by the Engineer. If the Contract does not require a finish HMA
wearing course, then the preleveling of uneven or broken surfaces
shall be accomplished by placing asphalt concrete of the class
specified with a motor patrol grader, by hand-raking, by Miller
box, or by such other method acceptable to the Engineer.
After placement, the preleveling Material shall be thoroughly
compacted with a pneumatic tire roller unless alternate Equipment
is approved by the Engineer.
When planing is not a Bid item in the Contract, the Contractor
shall be prepared to spot grind occasional high areas caused by
rutting, etc., to a depth to allow for a uniform application of
5-04.3(4)B3 PLANING BITUMINOUS PAVEMENT
5-04.3(4)B3a PRE-PLANING METAL DETECTION CHECK Before beginning
planing of pavements, and before any additional depth planning when
the Engineer, the Contractor shall conduct a physical survey of
existing pavement to be planed with Equipment that can identify
hidden metal objects.
Should such metal be identified, the Contractor shall promptly
bring this to the attention of the Engineer.
See Section 1-07.16(1) regarding the protection of survey
monumentation that may be hidden in pavement.
Any damage to Equipment resulting from the Contractors failure
to conduct a pre-planing metal detection survey, or from the
Contractors failure to bring to the attention of the Engineer any
hidden metal that is detected, shall be the Contractors sole
Also see Section 5-04.3(17) regarding a planing plan and
pre-planing briefing prior to beginning planing.
5-04.3(4)B3b PLANING See Section 5-04.3(17) regarding a planing
plan, and pre-planing briefing prior to beginning planing Locations
of existing surfacing to be planed will be indicated in the
Contract. Where planing an existing pavement is specified in the
Contract, the Contractor shall be prepared
to both remove existing surfacing material, and to reshape a
surface to remove irregularities. The finished product shall be a
prepared surface acceptable for receiving an HMA overlay.
Planing shall be by the cold milling method unless otherwise
specified in the Contract. The planer shall not be used on the
final wearing course of new HMA.
Planing operations shall be conducted in a manner that does not
tear, break, burn, or otherwise damage the surface which is to
remain. The finished planed surface shall be slightly grooved or
roughened and shall be free from gouges, deep grooves, ridges, or
other imperfections. Repair of the surface to remain that is
damaged by the Contractors planing shall be by a method acceptable
to the Engineer.
Metal castings and other surface improvements damaged by planing
shall be repaired or replaced as determined by the Engineer.
A tapered wedge cut shall be planed longitudinally along curb
lines sufficient to provide a minimum of 4 inches of curb reveal
after placement and compaction of the final wearing course. The
dimensions of the wedge shall be as shown on the Drawings or as
specified by the Engineer.
A tapered wedge cut shall also be made at transitions to
adjoining pavement surfaces (meet lines) where butt joints are
indicated on the Drawings. Butt joints shall be cut in a straight
line with vertical faces 2 inches or more in height and shall
produce a smooth transition to the existing adjoining pavement.
After planing is complete, the planed surfaces shall be swept,
cleaned, and if required by the Contract, patched and
The Engineer may direct additional depth planing. Prior to
performing this additional depth planing, the Contractor shall
first conduct a hidden metal in pavement detection survey as
required in Section 5-04.3(4)B3a.
5-04.3(4)B4 TACK COAT AND DISTRIBUTOR EQUIPMENT REQUIREMENTS
5-04.3(4)B4a TACK COAT REQUIREMENT Tack coat shall be CSS-1,
CSS-1h, or STE-1 emulsified asphalt. The CSS-1 and CSS-1h
emulsified asphalt may be diluted with water at a rate not to
exceed one part water to one part emulsified asphalt. The
emulsified asphalt shall not exceed the maximum temperature
recommended by the emulsified asphalt manufacturer.
A tack coat of asphalt, applied at the rate of 0.02 to 0.08
gallons per square yard of retained asphalt, shall be applied to
all paved surfaces on which any course of HMA is to be placed or
abutted. The tack coat shall cover the existing pavement uniformly
with a residual asphalt film free of streaks and bare spots.
The Contractor shall make arrangements with the Engineer
demonstrating tack coat application at the beginning of such
application. Once the Engineer approves the tack coat application
method and rate of application, the Contractor shall continue with
such application without exception.
Where the new asphalt concrete abuts a curb or gutter, cold
pavement joint, trimmed meet line, or any metal surface, tack coat
of asphalt shall be applied on the vertical face of the abutting
surface. The application on the contact surfaces shall be uniform
in order to avoid an accumulation of excess asphalt. Excess tack
coat shall be immediately removed. The Contractor shall not apply
the tack coat on vertical contact surfaces above the finished
height of the asphalt concrete being placed.
Tack coat shall be applied only to surfaces to receive tack coat
treatment, and shall not be applied to any other surface. Tack coat
applied to surfaces not to be coated shall require immediate
removal of the tack coat, including thorough cleaning of the
surface area as may be reasonably necessary for leaving no
Equipment shall not operate on tacked surfaces until the tack
has broken and cured. If the Contractors operation damages the tack
coat it shall be repaired prior to placement of the HMA. For
surfaces open to traffic, the application of tack coat shall be
limited to surfaces that will be paved during the same working
5-04.3(4)B4b DISTRIBUTOR EQUIPMENT REQUIREMENT The distributor
Equipment shall be capable of distributing a uniform tack coat in
controlled amounts. The distributor shall have a capacity of not
less than 1,000 gallons, and shall be so designed,
equipped, maintained, and operated that asphalt Material of an
even heat shall be uniformly applied at the required rate.
The power for operating the pressure pump shall be supplied by a
power unit which provides a uniform spray from each of the nozzles
across the spray bar and extensions.
In addition, the distributor shall be equipped with the
following: 1. a thermometer to indicate the temperature of the tack
coat material, 2. a thermometer installed permanently in the tank
to indicate temperatures at all times, 3. hand operated spray
Equipment for use only on inaccessible and irregularly shaped
areas, 4. a 10-foot spray bar with extensions, 5. pressure pump
and gauge, and volume gauge so located as to be observed easily by
Engineer from the ground, and 6. a tachometer to control
accurately the speed and spread of asphalt. The Engineer may allow
hand operated spray Equipment separate from the distributor
for inaccessible and irregularly shaped areas if the Contractor
can demonstrate acceptable tack coat application.
5-04.3(4)C SURFACE PREPARATION OF UNTREATED SURFACES
5-04.3(4)C1 GENERAL Untreated roadway surfaces, including
intersections and side roadway approaches which are to
receive asphalt concrete pavement, or other surfacing (see
Sections 4-04 and 5-02), shall be shaped to a uniform grade and
cross-section, conforming as nearly as possible to that which
Where new lines and grades are indicated in the Contract or
staked by the Engineer. The basis for establishing final line and
grade in such cases shall be curbs, curbs and gutters,
existing pavement, or pavement edges or other existing street
improvements. Existing driveways shall be graded as necessary to
provide a smooth transition to the final grade of the new pavement
surface including such grading as may be necessary to permit
Where no curbs or curbs and gutters exist and where none are
required by Contract, subgrade preparation shall extend one foot on
each side of the roadway beyond the final asphalt paving width
indicated on the Drawings. The Contractor shall be prepared to
extend this subgrade preparation to such greater width as the
Engineer may require to accommodate local conditions such as
The grade shall be shaped so that all frame castings for
manholes, monument boxes, gate valve boxes, catch basins, etc.
within the roadway section to be treated, extend above the prepared
surface, and such that all castings are flush with the final
wearing course. Where existing asphalt or Portland cement concrete
pavement is being met with new asphalt surfacing, sufficient
existing untreated surfacing shall be removed to permit the forming
of a butt joint. The completed finish surface, including castings
and transitions with existing treated surfaces, shall be smooth as
specified in Section 5-04.3(12).
Those areas and surfaces which are to be prepared for the
placement of asphalt concrete pavement or other surfacing shall be
considered Subgrade for the new construction. See Section 2-06 for
subgrade preparation requirements. Excess native material deemed
suitable by the Engineer shall be considered selected Material per
Section 2-03.3(10) and shall be stockpiled by the Contractor or
bladed to the roadway edge and used as needed for fill or shoulder
restoration following completion of the paving. The selected
Material shall be used to the fullest extent possible as sub-base
Material prior to the placement of new crushed rock.
Water shall be available on site and shall be applied as
necessary to meet compaction requirements and to alleviate
Excess material shall be disposed of.
5-04.3(4)C2 PRIME COAT TREATMENT Where required in the Contract,
a prime coat treatment of asphalt complying with the
of Section 5-02.3(3) for existing gravel, crushed rock, or oil
mat streets shall be applied prior to paving with asphalt concrete.
The prime coat shall be applied over the entire area of proposed
asphalt pavement construction. Following the application of the
prime coat, HMA shall not be placed until the prime coat has
In the event the surface receiving the prime coat is of such
gradation and relative density as to resist penetration of the
prime coat, the Contractor shall immediately before application of
the prime coat, loosen no more than the upper 1/2 inch of surface
and regrade it without compaction.
The Contractor shall maintain the completed prime coat by
blading or brooming until the asphalt concrete is placed. Should
any holes, breaks, or irregularities develop in the roadway surface
after the prime coat has been applied, such defects shall be
patched or repaired in accordance with Section 5-04.3(4)C1
immediately in advance of placing the asphalt concrete
Immediately prior to placing the HMA, the surface of the prime
coat shall be swept clean of all dirt, dust, and other foreign
5-04.3(4)D CRACK SEALING Where the Contract requires Crack
Sealing, all cracks and joints shall be cleaned with a stiff-
bristled broom and compressed air. Loose pieces shall be removed
and disposed of. After cleaning, all cracks less than 1/4 inch in
width shall be filled with straight CSS-1 emulsified
asphalt and topped with sand. After cleaning, all cracks and
joints at least 1/4 inch or greater in width, shall be filled with
slurry. Rubberized asphalt shall be used where specified in the
Contract. The Contractor may request substitution of rubberized
asphalt for sand slurry; however, such
request requires written approval from the Engineer before use.
Rubberized asphalt shall not be used to seal cracks greater than
1-1/2 inches in width.
Application of the sand slurry or rubberized asphalt shall be as
1. Sand Slurry: The sand slurry shall consist of 20 percent
CSS-1 emulsified asphalt, 2 percent Portland cement, sufficient
water for workability, and the remainder clean U.S. No. 4-0 paving
sand. The components shall be thoroughly mixed and poured into the
cracks and joints until full. The following day, any cracks or
joints that are not completely filled shall be topped off with
additional sand slurry. After the sand slurry is placed, the filler
shall be struck off flush with the existing pavement surface and
allowed to cure. The HMA overlay shall not be placed until the
slurry has fully cured. 2. Rubberized Asphalt: The sealant Material
shall meet the requirements of Section 9-04.10 and shall be applied
in accordance with the sealant manufacturers recommendations. These
recommendations shall be submitted to the Engineer by the
Contractor prior to the start of this type construction and shall
include recommended heating time and temperature, allowable storage
time and temperatures after initial heating, allowable reheating
criteria, and application temperature range. The cracks shall be
completely dry before being filled with the rubberized asphalt.
Filling shall be controlled to confine the Material within the
crack or joint. Where the sealed cracks are to be overlaid with
asphalt, the sealant shall be recessed 3/8 inch below the surface.
The Contractors method of sealant application shall confine the
sealant to the crack or joint and shall not result in any spillage
on the pavement surface.
Should spillage occur, the Contractor shall have readily
available, Supplies and as necessary to timely and effectively
remove sealant over-application.
5-04.3(5) HEATING OF ASPHALT BINDER The temperature of the
asphalt binder shall not exceed the asphalt binder
recommended maximum temperature at any time, and shall not fall
below the minimum temperature recommended by the asphalt binder
manufacturer. The asphalt binder shall be heated in a manner that
prevents local variations in heating. The heating method shall
provide a continuous supply of asphalt binder to the mixer at a
uniform average temperature with no individual variations exceeding
25F. Also see Section 5-04.3(2) regarding HMA mixing plant
5-04.3(6) HMA MIX DESIGN AND SUBMITTAL REQUIREMENTS
5-04.3(6)A PREPARATION OF AGGREGATES Sufficient storage space
shall be provided for each size of aggregate. The aggregates shall
removed from stockpile(s) in a manner to ensure a minimum of
segregation when being moved to the HMA plant for processing into
the final mixture. Different aggregate sizes shall be kept
separated until they have been delivered to the HMA plant.
5-04.3(6)B MIX DESIGN
5-04.3(6)B1 GENERAL From the stockpiled aggregates to be used in
the production of HMA, the Contractor shall
determine a design aggregate structure and asphalt binder
content in accordance with WSDOT Standard Operating Procedure 732,
Volumetric Design for Hot-Mix Asphalt (HMA), available in the
current edition of the Washington State Department of
Transportations Materials Manual M 46-01. The grade of asphalt
binder shall be as specified in the Contract (also see Section
5-04.2(1) where binder substitution is allowed). The nominal
maximum aggregate size and design ESALs shall be as required by the
Contract. The amount of anti-stripping additive to be added to the
mix will be determined by the Engineer based on the Contractors
proposed design and submittal (see below and Section 9-02.4).
Once the Contractor has determined the aggregate structure and
binder content, the Contractors submittal shall provide data
demonstrating that the proposed HMA design meets the requirements
of Sections 9-03.8(2) and 9-03.8(6). In no case shall the HMA
paving begin before the determination of anti-stripping agent
requirement by the Engineer has been made.
5-04.3(6)B2 APPLICATION DEFINITIONS Unless the Contract
specifies otherwise, the following definitions shall be used
regarding HMA Cl
mix designs and apply to all HMA submittals: Structural
application major quantity: an HMA Cl mix used for vehicular
traffic where the
Project specifies not less than 400 tons of HMA. See Section
5-04.3(6)C for submittal requirements.
Structural application - minor quantity: an HMA Cl mix used for
vehicular traffic where the Project specifies less than 400 tons of
HMA See Section 5-04.3(6)D for submittal requirements.
Non-structural application: an HMA Cl mix used for sidewalks,
ditches, slopes, paths, trails, gores and other non-vehicular
traffic application. See Section 5-04.3(6)E for submittal
For any quantity structural application, vehicular traffic shall
include roadways of any kind for vehicular traffic, alleys,
driveways, and other surfaces as may be specified in the
5-04.3(6)C SUBMITTAL STRUCTURAL APPLICATION MAJOR QUANTITY
5-04.3(6)C1 GENERAL As a convenience to accommodate accelerated
submittals for future uses of an Engineer approved
HMA Cl mix design major quantity structural application, an
Engineer approved HMA Cl major quantity structural application mix
design shall remain approved for use on all future Projects with a
Bid Opening Date within 365 consecutive calendar days from the date
of approval of that specific HMA Cl mix. The SPU Materials
Laboratory will specify the approval date on the returned
submittal, and will maintain records on such. On future Contracts,
the Contractor shall contact the SPU Materials Laboratory
(206-386-1236) to find out if and when a specific major quantity
structural application mix design has been Engineer approved.
5-04.3(6)C2 MIX DESIGN AND SAMPLE SUBMITTAL REQUIREMENTS For HMA
Cl mix designs not approved by the Engineer as specified in Section
Contractors HMA Cl submittal shall require 20 Working Days and
requires both the Contractor mix design and samples.
The following Contractor mix design information shall be
submitted for each HMA class: 1. Project name and Public Works (PW)
number. 2. HMA class designation and HMA Supplier. 3. Contractors
mix design number, or other designating identification
(designation). 4. Design equivalent single axle loads (design
ESALs). 5. Aggregate source (also see Sections 1-06.1 and 1-08.3(2)
item 6). 6. Aggregate gradations, including blending ratio. 7.
Percent (by weight of final mix) of RAP used. 8. Target gradation
of final HMA mix. 9. 0.45 power plot of target gradation showing
aggregate gradation control points zone. 10. Binder source and
performance grade (e.g. PG xx-yy). 11. Temperature Viscosity curve
of the binder. 12. Recommended binder compaction temperature range.
13. Recommended binder mixing temperature range. 14. Maximum
allowable binder temperature. 15. Type and brand of anti-stripping
additive. 16. Binder content of RAP (percent by weight of RAP). 17.
Percent (by weight of final mix) of binder in final mix (Pb). 18.
Effective Binder Content (Pbe). 19. HMA compaction temperature for
the gyratory compactor. 20. Relative density of the final mix at
Ndesign gyrations. 21. Number of design (Ndesign) gyrations used
(Nini; Ndes; Nmax). 22. Voids in Mineral Aggregate (VMA). 23. Voids
filled with asphalt (VFA). 24. Air voids in the compacted mixture
(Va). 25. Dust/Asphalt Ratio. 26. Sand Equivalent of the aggregate
fraction passing U.S. No. 4 sieve. 27. Percent of flat and
elongated particles retained on the U.S. No. 4 sieve. 28.
Theoretical maximum density of the mix (Gmm). 29. Percent of Gmm
for extruded specimens at Nini, Ndes and Nmax. 30. Bulk specific
gravity of the extruded specimen at Ndesign gyrations (Gmb) 31.
Bulk specific gravity of the combined aggregates in the mix (Gsb).
32. Effective specific gravity of the combined aggregates in the
mix (Gse). 34. Bulk specific gravity of the aggregate fraction
passing the 3/8 sieve. 35. Bulk specific gravity of the aggregate
fraction retained on the 3/8 sieve. 36. Specific gravity of the
binder (Gb). Samples: The mix design submittal shall be accompanied
with the following minimum sized
samples: 1) The HMA class mix (if RAP is proposed, the mix shall
contain the RAP) 75
pounds, 2) Asphalt binder(s) 1 quart 3) Recycled asphalt
pavement component (RAP), if used 25
pounds 4) Anti-stripping agent 1 quart Any adjustment to an
Engineer approved HMA class JMF will require a submittal (Section
05.3(5)) and the approval of the Engineer per Section
Submittal of items 2. through 4. (not 2) through 4)) above may
be waived by the Engineer if the Contractor submits a valid and
current WSDOT mix design of the same class of HMA utilizing the
same constituents from the same sources as the proposed mix design
including anti-stripping agent.
The Contractor may propose an asphalt binder from a secondary
source in the same submittal as the primary binder source, and
shall make this known in the submittal (see items 10, 11, 12, 13,
16, 17, 18, and 36).
Based on the submittal proposed by the Contractor, the Engineer
will determine the anti-stripping additive requirement, and will
make this information known on the returned submittal.
If the Engineer determines the submitted mix design is
defective, the Engineer will provide Written Notice identifying
such defect as may apply.
The Contractor shall not commence production of any HMA class
until that HMA JMF mix design has been established and approved by
Any change in source of supply for any of the constituents of an
approved HMA class JMF will require a new mix design be submitted
and approved prior to use as specified in this Section.
If the results of the verification testing by the Engineer of
the submitted sample Materials and proposed mix design meet the
requirements of Sections 9-02.1(4) and 9-03.8, then the submittal
will be considered approved. The approved mix design will be the
initial job mix formula (JMF) for the specified HMA class of mix
and an Engineer approval date will be assigned.
To aid the Contractor in preparing the HMA mix design submittal,
the Contract will contain an HMA Mix Design Submittal form located
in the Appendix of the Project Manual.
5-04.3(6)C3 ACCELERATED SUBMITTAL When an Engineer approved HMA
Cl mix design for major quantity structural application is
specified in the Contract and this HMA mix is within the 365
calendar Day window before the Bid Opening Date, the Contractor
shall submit to the Engineer at least 5 Working Days in advance, a
Manufacturers Certificate of Compliance stating the following:
1. For each HMA class specified in the Contract, the name and
location of each Supplier providing the Engineer approved HMA class
mix and component parts.
2. Suppliers HMA Cl mix design number, or other designating
identification (designation) consistent with the Engineer approved
HMA class mix.
5-04.3(6)C4 CERTIFICATION TO ACCOMPANY HMA DELIVERY For any HMA
class major quantity structural application mix, each delivery of
HMA Cl to the Project
Site shall be accompanied with a certification stating the
following: 1) The HMA mix being delivered is an Engineer approved
HMA mix, 2) Name and location of HMA Cl Supplier, 3) Suppliers HMA
Cl mix identification number, 4) Date and time of load out, 5)
Class of HMA, 6) Grade of binder, 7) Percent (by weight of binder)
of anti-stripping agent, and 8) Tonnage of HMA in the hauling
5-04.3(6)D STRUCTURAL APPLICATION - MINOR QUANTITY For HMA Cl
minor quantity structural application mixes, the Contractor shall
submit at least 5
Working Days in advance of first use, a Manufacturers
Certificate of Compliance showing items (1) through (7) below.
At the request of the Engineer, the Contractor shall submit the
approved mix design data previously submitted and approved in
The Engineer reserves the right to obtain samples of a
previously approved HMA Cl mix and/or its individual constituents
for verification of the mix design.
In addition, every delivery of the HMA Cl mix to the Project
Site shall be accompanied with a certificate stating the
(1) Name and location of HMA Supplier, (2) Suppliers HMA mix
identification designation, (3) Date and time of load out, (4)
Class of HMA, (5) Binder grade of PG 64-22, (6) Percent (by weight
of binder) of anti-stripping agent including brand name and type,
(7) Minimum design ESALs of 10,000,000, and (8) Tonnage in
5-04.3(6)E NON-STRUCTURAL APPLICATIONS For HMA Cl non-structural
application mixes, the Contractor shall submit at least 5 Working
advance of first use, a Manufacturers Certificate of Compliance
showing items (1) through (3) below.
At the request of the Engineer, the Contractor shall submit the
approved mix design data specified in Section 5-04.3(6)C3.
The Engineer reserves the right to obtain samples of a
previously approved HMA Cl mix and/or its individual constituents
for verification of the mix design.
In addition, every delivery of the HMA Cl mix to the Project
Site shall be accompanied with a certificate stating the
(1) HMA Class Inch, (2) Binder grade of PG 64-22 (binder grade
may be substituted as described in Section 5-
04.2(1)), (3) Supplier designed at any ESAL level, and (4)
Tonnage in hauling vehicle.
5-04.3(7) HMA MIXING PROCESS
5-04.3(7)A GENERAL After the required amounts of Mineral
Aggregate and asphalt binder have been introduced into the
mixer, the HMA shall be mixed until a complete and uniform
coating of the particles and a thorough distribution of the asphalt
binder throughout the Mineral Aggregates is ensured.
When discharged, the temperature of the HMA shall not exceed the
maximum temperature recommended by the asphalt binder
A maximum water content of 1 percent in the HMA, at discharge,
will be allowed providing the water causes no problems with
compaction, handling, stripping, or flushing. If the water content
in the HMA causes any of these problems, the HMA will be considered
defective Material. The Contractor shall stop production of the HMA
and discontinue the placing of HMA. As specified in Section 1-05.7,
the Contractor shall provide a remedy acceptable to the Engineer
addressing the water content of the HMA. Defective Material in
place shall be removed and replaced with Material that meets the
Storing or holding of the HMA in approved storage facilities
will be permitted during the daily operation but in no event shall
the HMA be held for more than 24 hours. HMA held for more than 24
hours after mixing will be rejected. Rejected HMA shall be disposed
of by the Contractor at no expense to the Owner. The storage
facility shall have an accessible device located at the top of the
cone or about the third point from the top. The device shall
indicate the amount of material in storage. No HMA shall be
accepted from the storage facility when the HMA in storage is below
the top of the cone of the storage facility, except as the storage
facility is being emptied at the end of the working shift.
Where HMA has been held in approved storage and no load out has
occurred for 4 continuous hours, then the first 4 tons to be loaded
out of the storage facility shall be wasted and disposed of at the
5-04.3(7)B ACCEPTANCE SAMPLING AND TESTING HMA MIXTURE
Acceptance of HMA will be based on the following: 1. Aggregates.
The acceptance criteria for aggregate properties of sand
equivalent, flat and
elongated, fine aggregate angularity and fracture will be their
conformance to the requirements of Section 9-03.8(2).
2. Hot Mix Asphalt Mixture. The acceptance criteria for the HMA
mixture shall be as specified in Section 9-03.8(7), HMA Tolerances
and Adjustments. A. Sampling
1. No samples will be obtained from either the first or last 25
tons of HMA produced in each production shift.
2. Samples for acceptance testing will be obtained on a random
basis at the point of delivery in accordance with AASHTO T168.
B. Definition of Sampling Lot and Sublot A lot is defined as a
discrete quantity of as-constructed pavement to which an acceptance
procedure is applied. For the purpose of acceptance sampling and
testing, a lot is defined as the total quantity of Material or work
produced for each job mix formula (JMF) placed. A lot is
represented by randomly selected samples that will be tested for
acceptance. Only one lot per JMF is expected. The initial JMF is
defined in Section 5-04.3(7)A, Mix Design. The Contractor may
request a change in the JMF in accordance with Section 9-03.8(7).
If the request is approved, all of the Material produced up to the
time of the change will be evaluated on the basis of tests on
samples taken from that JMF and a new lot will begin.
Sampling evaluation will be performed on a random basis at the
frequency of one sample per sublot. Sublot size will be determined
to the nearest 100 tons to provide not less than two uniform sized
sublots, based on proposal quantities, with a maximum sublot size
of 400 tons. Sampling and testing will be performed on a random
basis as determined by the Engineer. The quantity of material
represented by the final sublot may be increased to a maximum of 2
times the sublot quantity calculated.
C. Test Results The Engineer will furnish the Contractor with a
copy of the results of the acceptance testing performed in the
Sublot sample test results may be challenged by the Contractor.
To challenge the Laboratorys test results, the Contractor shall
with the requirements of Section 1-04.5. Resolution of this
challenge shall be by a split of the original acceptance
sample that will be retested by the Owners Laboratory. The split
of the sample with challenged results will not be tested by the
same tester that conducted the original acceptance test. The
challenge sample will be tested for a complete gradation analysis,
for asphalt binder content, and for percent air voids (Va). The
results of the challenge sample will be compared to the original
results of the acceptance sample test and evaluated according to
the following criteria:
Deviation from JMF Property Allowable deviation (%) Standard
Specification Reference U.S. No. 4 and larger sieves 4.0 % for each
sieve 9-03.8(6) U.S. No. 8 sieve 2.0 % 9-03.8(6) U.S. No. 200 sieve
0.4 % 9-03.8(6) Asphalt binder content 0.3 % 5-04.3(6)C1, item 18
Air Voids in the Compacted Mixture (Va)
0.7 % 5-04.3(6)C1, item 24
If the results of the challenge sample testing are outside the
allowable deviation established above for any of the above
parameters, the Contractor agrees the sublot is defective and that
the sublot shall be removed and replaced and the cost of retesting
be deducted at the rates published in Section 1-05.7 from any
monies due or that may come due the Contractor under the Contract.
If the results of the challenge sample testing are within all
parameters established above, the sublot will be accepted and the
cost of retesting will be the Owner's responsibility. D. Test
Testing of HMA for compliance of volumetric properties (VMA, VFA
Va and Dust/Asphalt Ratio) will be by WSDOT SOP 731, Method for
Determining Volumetric Properties of Asphalt Concrete Pavement
Class Superpave. WSDOT FOP for AASHTO T 166, Bulk Specific Gravity
of Compacted Bituminous Mixtures Using Saturated Surface-Dry
Specimens. WSDOT FOP for AASHTO T 209 FOP for Theoretical Maximum
Specific Gravity and Density of Bituminous Paving Mixtures Rice
Density. Testing for compliance of asphalt binder content will be
by WSDOT FOP for AASHTO T 308, Determining the Asphalt Binder
Content of Hot Mix Asphalt (HMA) by the Ignition Method. WAQTC FOP
TM 6, Moisture Content of Bituminous Mixtures by Oven. Testing for
compliance of gradation will be by WAQTC FOP for AASHTO T 27/T 11.
E. Reject Mixture
1. Rejection by Contractor: The Contractor may, prior to
sampling, elect to remove any defective Material and replace it
with new Material. Any such new Material may be sampled, tested,
and evaluated for acceptance.
2. Rejection by Engineer: Sublots found to be defective during
acceptance sampling and testing shall be removed and replaced. In
addition, the Engineer may also isolate and reject within a sublot
any Material that is determined to be defective.
If, during paving, the Engineer determines Material being placed
does not meet Specification, the Contractor shall shut down
operations and shall not resume HMA placement until such time as
the Engineer is satisfied that specified Material is being
The Engineer may, without sampling, reject any batch, load, or
section of HMA that appears defective in gradation, temperature or
asphalt binder content. Material rejected before placement shall
not be incorporated into the pavement. Any rejected HMA section of
roadway shall be removed. The Contractor may request that the
rejected Material be tested. If the Contractor elects to have the
rejected Material tested, a minimum of three representative samples
will be obtained and tested. Acceptance of rejected Material will
be based on conformance with the Specifications. No payment will be
made for Material that fails to meet Specification. In addition,
the cost of sampling and testing shall be borne by the Contractor.
If the Material meets Specification, the cost of sampling and
testing will be borne by the Owner and payment for the HMA will be
made at the Bid item price.
5-04.3(8) SPREADING AND FINISHING The mixture shall be laid upon
an approved surface, spread, and struck off to the grade and
elevation established. HMA paving Equipment complying with
Section 5-04.3(3)B shall be used to distribute the mixture.
A material transfer vehicle (MTV) shall be used on any paving
operation where the daily placement exceeds 800 tons. Should a
specific application arise where an MTV is not suitable, the
Contractor shall submit a request for a waiver to the Engineer with
explanation. The Engineers approval is required for not using an
MTV when daily placement is expected to exceed 800 tons.
Unless otherwise directed by the Engineer, the nominal compacted
depth of any layer of any course shall conform to the following
Material Maximum HMA Class 1" 0.35 feet HMA Class 3/4" 0.30 feet
HMA Class 1/2" 0.25 feet HMA Class 3/8" 0.10 feet
When more than one course is necessary to meet the final paving
grade, the first course shall include any widening of the existing
roadway and preleveling of the existing pavement surface. The
preleveling course or courses shall be constructed so that the
final wearing course has a uniform compacted depth and conforms to
the finished grade and cross section elevations specified.
Construction of one course upon another shall not proceed until the
underlying course has cooled and set.
On areas where irregularities or unavoidable obstacles make the
use of mechanical spreading and finishing Equipment impractical,
the paving may be done with other approved Equipment or by
When more than one JMF is being utilized to produce HMA, the
Material produced for each JMF shall be placed by separate
spreading and compacting equipment. The intermingling of HMA
produced from more than one JMF is prohibited. Each strip of HMA
placed during a working shift shall conform to a single JMF
established for the class of HMA specified unless there is a need
to make an adjustment in the JMF. No adjustment to the JMF will be
allowed without approval of the Engineer.
When laying HMA, the paver shall be operated at a uniform
forward speed consistent with the trucking delivery rate and roller
train capacity to result in a continuous operation. The auger speed
and flight gate opening shall be adjusted to coordinate with the
During mainline paving, the wings on the receiving hopper shall
not be folded, and the mix level in the hopper shall be maintained
so that the conveyors are not exposed, unless the Engineer approves
Manual operation of the screed will be permitted in the
construction of irregularly shaped and minor areas. These areas
include, but are not limited to, gore areas, road approaches,
tapers and left-turn channelizations.
When specified in the Contract, reference lines for vertical
control will be required. Lines shall be placed on both outer edges
of the traveled way of each roadway. Horizontal control utilizing
the reference lines will be permitted. The grade and slope for
intermediate lanes shall be controlled automatically from reference
lines, or by means of a mat referencing device and a slope control
device. When the finish of the grade prepared for paving is
superior to the established tolerances and when, in the opinion of
the Engineer, further improvement to the line, grade,
cross-section, and smoothness can best be achieved without the
of the reference line, a mat referencing device may be
substituted for the reference line. Substitution of the mat
referencing device will be subject to the continued approval of the
Engineer. The reference line may be removed after the completion of
placing the first course of HMA when approved by the Engineer.
Whenever the Engineer determines that any of these methods are
failing to provide the necessary vertical control, the reference
lines shall be promptly reinstalled by the Contractor before
further placement of HMA.
5-04.3(8)A UTILITY ADJUSTMENTS Utility castings shall be
adjusted to finished grade prior to the construction of the final
course as described Section 7-20.
5-04.3(9)A GENERAL Immediately after the HMA has been spread and
struck off, and after surface irregularities have
been adjusted, the mix shall be thoroughly and uniformly
compacted. The completed course shall be free from ridges, ruts,
humps, depressions, objectionable marks, and irregularities and
shall conform to the line, grade, and cross-section shown in the
Drawings If necessary, the JMF may be altered in accordance with
Section 9-03.8(7) to achieve desired results.
Compaction shall take place when the mixture is in the proper
condition so that no undue displacement, cracking, or shoving
occurs. All compaction equipment shall be capable of producing the
required compaction. Areas inaccessible to large compaction
equipment shall be compacted by mechanical or hand tampers. Any HMA
that becomes loose, broken, contaminated, shows an excess or
deficiency of asphalt, or is in any way defective, shall be removed
and replaced at no additional cost with fresh material which shall
be immediately compacted to conform with the surrounding area.
The type of rollers to be used and their relative position in
the compaction sequence shall generally be the Contractors option,
provided Specification densities are attained. An exception shall
be that pneumatic tired rollers shall be used between October 1st
of any year and April 1st of the following year unless the Engineer
directs otherwise. Coverages with a vibratory or steel wheel roller
may precede pneumatic tired rolling.
Vibratory rollers shall not be operated in the vibratory mode
when the internal temperature of the mix is less than 175F.
Regardless of mix temperature, a vibratory roller shall not be
operated in a vibratory mode when checking or cracking of the mat
occurs. Vibratory rollers in the vibratory mode are prohibited on
bridge decks, brick bases, and cobblestone bases.
HMA for preleveling shall be thoroughly compacted to the
satisfaction of the Engineer.
5-04.3(9)B1 COMPACTION REQUIREMENT For an HMA Cl having a
specified compacted course thickness greater than 0.10 foot,
acceptable level of relative density shall be a minimum 92.0
percent of the reference maximum density. The reference maximum
density will be determined by the Engineer as the moving average of
the most recent three determinations for the JMF being placed to
accommodate start-up for a large placement. Where less than three
determinations have been made, the reference maximum density will
be the average of all determinations made to that time to
accommodate start-up for a large placement. The actual density
attained for a sublot of an HMA Cl will be determined as the
average of five nuclear density gauge tests (after completion of
the finish rolling) at randomly selected locations within each
density sublot. In addition to the randomly selected locations, the
Engineer may select any additional location(s) for testing that
appears to be deficient or in any way defective. Such additional
tests shall be included in the in the calculation of the average
density for that sublot. The quantity represented by each sublot
for density testing will be no greater than a single days
production or 400 tons, whichever is less. For density testing of
very large daily placements of HMA, the Engineer may increase the
size of the final sublot to a maximum of 600 tons. A lot shall be
as defined 5-04.3(7)B.
5-04.3(9)B2 TEST RESULTS Density sublots not meeting the
prescribed minimum relative density shall be considered
work, and shall be removed and replaced. No payment will be made
for defective Material that fails to meet the minimum relative
For compaction lots subject to rejection, cores may be used as
an alternate to the nuclear density gauge tests. When cores are
taken by the Engineer at the request of the Contractor, they shall
be requested by no later than 12:00 AM of the next Working Day
after receiving the test results. The cores will be taken at
locations selected by the Engineer. Cores shall not be located in
wheel paths. On sublots which
fail to attain the minimum relative density, the cost for the
coring will be deducted from any monies due or that may become due
the Contractor under the Contract at the rates published in Section
In addition to the randomly selected locations for relative
density tests for a sublot, the Engineer may also isolate any area
that is suspected of being defective in relative density. The
isolated area will be evaluated as a separate subsublot. Such
isolated area determinations shall be at the sole discretion of the
5-04.3(10)A LONGITUDINAL AND TRANSVERSE JOINTS The placing of
the top or wearing course shall be as nearly continuous as
possible, and the roller
shall pass over the unprotected end of the freshly laid mixture
only when the laying of the course is discontinued for such length
of time as to permit the mixture to become chilled. When this work
is resumed, the previously compacted mixture shall be sawcut back
to produce a slightly beveled edge for the full thickness of the
Where a transverse joint is being made and pavement will be open
to traffic, a temporary wedge of HMA shall be constructed of a 5:1
H:V slope. The HMA in the temporary wedge shall be separated from
the permanent HMA by strips of heavy wrapping paper. When paving
operations are renewed, the wrapping paper shall be removed and the
joint trimmed to a slightly beveled edge for the full thickness of
the new HMA course. The Material which is cut away shall be
disposed of and new mix shall be laid against the fresh cut.
Rollers or tamping irons shall be used to seal the joint.
All joints shall be flush and provide a smooth transition across
the meet line. The longitudinal joint in any one layer shall be
offset from the layer immediately below by not more
than 6 inches nor less than 2 inches. All longitudinal joints
constructed in the top layer shall be at a lane line or edge line
of the traveled way. Where traffic conditions, Project geometry or
other condition exist that make the construction of longitudinal
joints at the lane line or edge of the traveled way impractical or
impossible, a longitudinal joint may be constructed at the center
of the traffic lane with the Engineers written approval.
Hot lap joints may be allowed by the Engineer provided planned
grades are maintained, no surface irregularities exist and
compaction requirements are met. Two paving machines shall be used
to construct longitudinal hot lap joints; a minimum average
compacted density in accordance with 5-04.3(10) shall be achieved
throughout the traffic lane; and construction Equipment other than
rollers shall not operate on any uncompacted mix.
Immediately following the compaction of the top wearing course,
meet line joints where the new asphalt concrete abuts existing
asphalt concrete pavements, Portland cement concrete pavements, oil
mats, concrete curbs and gutter, etc., shall be sealed per Section
5-04.3(10)B NEW PAVEMENT CONNECTIONS WITH EXISTING PAVEMENTS
Where construction of new asphalt concrete pavement connects with
an existing roadway surface,
driveway, bridge, railway crossing, gutter, or other similar
facility, the Contractor shall provide a smooth riding transition
between the new surface and existing surface. Such work may require
the modification of the existing roadway profile by burning,
planing or milling in order to achieve the desired smooth riding
transition or may require other adjustment of the new connecting
Where butt joints are required at the meet lines of new
construction and existing surfaces, the existing abutting pavement
shall be trimmed by chipping, planing, milling or such other
acceptable method in order to insure a minimum depth of 2 inches of
compacted asphalt concrete at the point of connection. Meet lines
shall be trimmed straight and the edges vertical. Waste Material
resulting from such trimming or chipping shall be disposed of by
the Contractor. Butt joints will be required only at locations
designated on the Drawings. Unless the existing roadway profile
requires modification by planing, all other connections shall be
made by shimming or feathering to provide the necessary smooth
Where the transition is to be made by shimming or feathering, it
shall be accomplished at the time the final course is being
constructed by raking out the oversize aggregate from the HMA class
being used. The Contractor shall not leave the asphalt open graded
when feathering and shimming down to an existing surface. If
approved by the Engineer, shimming and feathering may be
accomplished at a later date. In such case, structural HMA Class
3/8 Inch shall be used.
Surfaces to be in contact with the new asphalt shall be tacked
in accordance with Section 5-04.3(4)C2.
Meet lines between new and existing surfaces shall be sealed
while the new asphalt concrete is still warm by painting with tack
coat and then immediately covering the asphalt paint strip with
clean, dry paving sand (mineral Aggregate Type 6) complying with
5-04.3(12) SURFACE SMOOTHNESS
5-04.3(12)A GENERAL The completed surface of all courses shall
be of uniform texture, be smooth, have a continuous
plane grade except across the crown. All surfaces shall be free
from defects of all kinds. The completed surface of the wearing
course shall not vary more than 1/8-inch from the lower edge of a
10-foot straightedge placed on the surface parallel to the
centerline. The transverse slope of the completed surface of the
wearing course shall vary not more than 1/4-inch in 10 feet from
the rate of transverse slope shown on the Drawings.
When deviations in excess of, but not more than twice, the above
tolerances are found, the pavement surface shall be corrected to
low places, or the removal of Material from high places by grinding
with an acceptable grinding machine. The corrected deviation shall
be sealed in accordance with Section 5-04.3(18). Where the Engineer
determines grinding or filling does not allow for an acceptable
repair, removal and replacement of the wearing course of asphalt
concrete will be required. Correction of defects shall be carried
out until there are no deviations greater than the allowable
All areas in which the surface of the completed pavement
deviates more than twice the allowable tolerances described above,
these areas shall be removed and replaced to the extents determined
by the Engineer.
However, if deviations are found which exceed the allowable
tolerances but are not in excess of twice the allowable tolerances
described above, and, in the opinion of the Engineer, correction by
means of any of the methods specified above do not produce
acceptable results as to smoothness and serviceability, the
Engineer may accept the completed pavement. Under these described
circumstances, the decision whether to accept the completed
pavement or to require corrections as described above shall be
vested entirely in the Engineer.
5-04.3(12)B CONCRETE OVERLAYING ASPHALT When Portland cement
concrete pavement is placed on asphalt concrete pavement, the
tolerance of the asphalt concrete pavement shall be such that no
elevation lies above the proposed finished grade minus the
specified depth of Portland cement concrete pavement. Prior to
placing the Portland cement concrete pavement, any such
irregularities shall be brought to the required tolerance by
grinding or other means acceptable to the Engineer.
5-04.3(15) WEATHER LIMITATIONS Asphalt for prime coat shall not
be applied when the ground temperature is lower than 50F
written approval of the Engineer. HMA shall not be placed on any
wet surface, or when the average surface temperatures are less
than those specified in the following table, or when weather
conditions otherwise prevent the proper handling or finishing of
the bituminous mixtures:
Surface Temperature Limitation Compacted Thickness (Feet)
Wearing Course Other Courses
Less than 0.10 55F 45F 0.10 to 0.20 45F 35F 0.21 to 0.35 35F
5-04.3(17) PAVING AND PLANING UNDER TRAFFIC
5-04.3(17)A GENERAL In addition the requirements of Section
1-07.23 and the traffic controls required in Section 1-10,
unless the Contract specifies otherwise or the Engineer agrees
to otherwise, the Contractor shall comply with the following:
1. Intersections: The Contractor shall keep intersections open
to traffic at all times, and shall comply with the traffic control
restrictions required by the Traffic Engineer. Each individual
intersection closure or partial closure, shall be addressed in the
Traffic Control Plan to be submitted to and approved by the
Engineer (see Section 1-10.2(5)).
When planing or paving and related construction must occur in an
intersection, the Contractor shall consider scheduling and
sequencing such work into quarters of the intersection, or half or
more of an intersection with side street detours. The Contractor
shall also be prepared to sequence the work to individual lanes or
Should closure of the intersection in its entirety be necessary,
and no trolley service is impacted, such closure shall be kept to
the minimum time required to place and compact the HMA mixture,
plane, remove asphalt, tack coat, and as needed.
Any work in an intersection shall include advance warning in
both signage and in Working Days advance notice as determined by
the Engineer, to alert traffic and emergency services of the
intersection closure or partial closure.
Work shall be scheduled so that consecutive intersections shall
not have construction in-progress at the same time. New compacted
HMA asphalt shall cool to ambient temperature before any traffic is
allowed on it. Traffic shall not be allowed on newly placed asphalt
until approval has been obtained from the Engineer.
2. Centerline marking, post-paving temporary marking, temporary
stop bars, and maintaining temporary pavement marking: The
Contractor shall comply with the requirements of Section
3. Permanent pavement marking: The Contractor shall comply with
the requirements of Section 8-22.3(1).
5-04.3(17)B SUBMITTALS - PLANING PLAN AND HMA PAVING PLAN The
Contractor shall submit a separate planing plan and a separate
paving plan to the Engineer at
least 5 Working Days in advance of each operations activity
begin date. These plans shall show, as to be discussed at the
pre-planing briefing and pre-paving briefing, how the moving
operation and traffic control are coordinated. When requested by
the Engineer, the Contractor shall provide each operations Traffic
Control Plan on 24 x 36 or larger size Shop Drawings with a scale
showing both the area of operation and sufficient detail of traffic
beyond the area of operation where detour traffic may be required.
The scale on the Shop Drawing shall be 1 inch = 20 feet, or may be
changed if the Engineer agrees sufficient detail is shown.
The planing operation and the paving operation includes, but is
not limited to, metal detection, removal of asphalt and temporary
asphalt of any kind, tack coat and drying, staging of supply
trucks, paving train(s), rolling, scheduling, and as may be
discussed at the briefing.
When intersections are to be partially or totally blocked, the
Contractor shall provide a minimum 2 Working Days in advance,
adequately sized and noticeable signage alerting traffic of
closures to come. The Traffic Control Plan shall show where Peace
Officers are to be stationed when signalization is to be, or may
be, countermanded, and show areas where flaggers are proposed.
At a minimum, the planing and the paving plan shall include the
following elements: 1. A copy of the approved traffic control plans
(per Section 1-10.2(5)) detailing each days
traffic control as it relates to the specific requirements of
that days planing, and paving. Briefly describe the sequencing of
traffic control consistent with the proposed planing and paving
sequence, and scheduling of placement of temporary pavement
markings and channelizing devices after each days planing, and
2. A copy of each intersections traffic control plan (see item 2
in Section 5-04.3(17)A). 3. Haul routes from Supplier facilities,
and locations of temporary parking and staging areas,
including return routes. The complete round trip shall be
described as it relates to the sequencing of paving operations.
4. Names of, and locations of HMA Supplier facility(ies) to be
used. 5. Listing of all Equipment to be used for paving. 6. Listing
of personnel and associated job classification assigned to each
piece of paving
Equipment. 7. Description (geometric or narrative) of the
scheduled sequence of planing and of paving,
and intended area of planing and of paving for each days work.
Such description shall include the directions of proposed planing
and of proposed paving, sequence of adjacent lane paving, sequence
of skipped lane paving, intersection planing and paving scheduling
and sequencing, and proposed notifications and coordinations to be
8. Names, job titles, and contact information for field, office,
and plant supervisory personnel.
5-04.3(17)C PRE-PAVING AND PRE-PLANING BRIEFING At least two (2)
Working Days before the first paving operation and the first
planing operation, and
as may be scheduled by the Engineer for future paving and
planing operations, to ensure the Contractor has
adequately prepared for notifying and coordinating as required
in the Contract, the Contractor shall be prepared to discuss that
days operations as they relate to other entities and the publics
safety and convenience, including driveway and business access,
garbage truck operations, Metro transit operations and working
around energized overhead wires, school and nursing home and
hospital and other accesses, other contractors who may be operating
in the area, pedestrian and bicycle traffic, emergency services,
and as may be applicable. The Contractor, and Subcontractors as may
be part of that days operations, shall meet with the Engineer and
discuss the proposed operation as it relates to the submitted
planing plan and paving plan, approved Traffic Control Plan, public
convenience and safety, and as may be necessary. Such discussion
shall include, but not be limited to:
1. General for both Paving Plan and for Planing Plan: A. The
actual times of beginning and ending daily operations; B. In
intersections, how break up the intersection, and address traffic
signalization for that operation including use of peace
officers; C. The sequencing and scheduling of paving operations and
of planing operations,
as applicable, as it relates to traffic control, to public
convenience and safety, and to other contractors who may operate in
the Project Site;
D. Notifications required of Contractor activities, and
coordinating with other entities and the public as may be
E. Describe the sequencing of installation and types of
temporary pavement markings as it relates to planing and to
F. Describe the sequencing of installation of, and the removal
of, temporary pavement patch material around exposed castings and
as may be needed;
G. Describe the procedures and Equipment to identify hidden
metal in the pavement (such as survey monumentation, monitoring
wells, street car rail, and castings) prior to planing (see Section
H. Describe how flaggers will be coordinated with the planing,
paving, and related operations;
I. Describe the sequencing of traffic controls for the process
of rigid pavement base repairs; and
J. Other items the Engineer may deem necessary to address. 2.
Paving - additional topics:
a) When begin applying tack and coordinating with paving; b) The
types of Equipment and numbers of each type Equipment to be used.
more pieces of Equipment than personnel are proposed, describe
the sequencing of the personnel operating the types Equipment.
Discuss the continuance of operator personnel for each type
Equipment as it relates to obtaining Specification
c) The number of JMFs to be placed and if more than one JMF, how
the Contractor ensures that the different JMFs are distinguished,
how pavers and MTVs are distinguished if more than one JMF is being
placed at the time, and how pavers and MTVs are cleaned so that one
JMF does not adversely influence the other JMF;
d) Describe contingency plans for that days operations such as
Equipment breakdown, rain out, and Supplier shutdown of
e) Number of sublots to be placed, sequencing of density
testing, and other sampling and testing.
5-04.3(18) SEALING OF PAVEMENT SURFACES Any wearing course or
other pavement course to be used for the driving surface will be
by the Engineer to determine whether a fog seal is required.
Determination will be made when the results of nuclear or core
density testing show that a seal is needed. The fog seal shall be
CSS-1 or CSS-1h emulsified asphalt uniformly applied to the
pavement. The finished application shall be free of streaks and
bare spots. The emulsified asphalt shall be diluted at a rate of
one part water to one part emulsified asphalt. The diluted
emulsified asphalt shall be applied at the rate of 0.10 to 0.18
(0.03 to 0.05 residual) gallons per square yard. The emulsified
asphalt shall be applied within the temperature range specified for
these asphalt emulsions in Section 5-02.3(3). Unless otherwise
approved by the Engineer, the fog seal shall be applied prior to
opening to traffic.
5-04.3(19) ANTI-STRIPPING ADDITIVE Anti-stripping additive shall
be added to the HMA in accordance with the Engineer determined
stripping additive requirement as made known on the returned
submittal (see Section 5-04.3(6)C)2.
5-04.3(20) SHOULDER PAVING Shoulders, if required, shall be
constructed to the lines, grades, and cross-sections specified.
Material for building up shoulders shall be Mineral Aggregate
5-04.3(21) NON-STRUCTURAL HMA APPLICATIONS
5-04.3(21)A HMA SIDEWALKS Asphalt walkways shall be constructed
at the locations and to the width specified on the Drawings.
Unless the Contract specifies otherwise, asphalt walkways shall
be constructed with a 4 inch section of compacted crushed rock
Mineral Aggregate Type 2 and covered with 3 inches of compacted HMA
5-04.3(21)B HMA DRIVEWAYS Asphalt driveways shall be constructed
as shown on the Drawings. Unless the Contract specifies
otherwise, the Contractor shall provide 3 inches of compacted
HMA of the class specified in the Contract over 4 inches of
compacted Mineral Aggregate Type 2.
5-04.3(23) TEMPORARY PAVEMENT PATCHING Unless the Contract
designates an HMA CL asphalt concrete as a temporary patch
temporary asphalt patch Material shall be in accordance with
Section 9-02.5. The Contractor shall furnish, place and maintain a
4 inch minimum compacted thickness of
temporary pavement patch Material over open cuts. Such temporary
asphalt patching will be required where vehicular or pedestrian
traffic must be accommodated and permanent pavement patching cannot
be placed immediately. Trench backfill shall be compacted as
specified in Section 7-17.3(3). Temporary pavement patch Material
shall be compacted and leveled to coincide with adjacent
In the event that the temporary surface subsides after the
initial placement, additional temporary pavement patch Material
shall be placed over the subsided Material as necessary to maintain
a surface level with existing pavement. The Contractor shall timely
maintain such temporary patching.
Prior to final restoration of the pavement, the Contractor shall
remove the temporary pavement patch Material and such underlying
material as may exist, clean the exposed face of the existing
pavement to remain, and restore the pavement.
5-04.4 MEASUREMENT Bid items of Work completed pursuant to the
Contract will be measured as provided in Section 1-
09.1, Measurement of Quantities, unless otherwise provided for
by individual measurement paragraphs herein this Section.
Measurement for HMA of the class specified will be by the ton
whether the HMA is used for structural or non-structural
applications, and whether a major quantity or a minor quantity. The
net weight of HMA being delivered to the Project Site shall be
weighed in the transporting Equipment on a certified platform
scale, and with accuracy, as specified in Section 1-09.2.
Measurement of HMA of the class specified will be based upon the
actual quantity incorporated into the Work as determined by the
Material load tickets received and accepted by the Engineer on the
day the Material was delivered and incorporated into the Work.
Deductions will be made for any asphaltic Material included in the
measurement that is not incorporated into the Work on the day
Measurement for Roadway Preparation will be made by a single
linear foot measurement along the centerline of the main roadway
being prepared. All related intersections, side street approaches,
and irregular shaped areas thereto will be incidental to this one
measurement. Measurement will be to the nearest whole linear
Measurement for Surface Preparation, Plane Bituminous Pavement
will be by the square yard and will be based on the average depth
shown on the Drawings plus any additional depth up to 4 inch
maximum to cover removal of high spots, to cover extra thickness
existing pavement, and to cover the extra depth required to provide
a 4 inch reveal along the curb line as specified in Section
5-04.3(4)B3b. Should the Drawings indicate or the Engineer order an
area be planed in excess of 4 inches, that area planed in excess of
4 inch total depth will be measured in additional square yards of
surface planed for up to an additional 4 inch depth. In general,
any area planed in excess of 4 inches will be measured by the
square yard for each incremental depth of 4 inches. The final
planed depth beyond the first 4 inch thickness will include
multiples of 4 inches with the last planing pass up to 4 inch
maximum. (Example an area of pavement planed to 9.5 inch total
depth will be measured as 3 times the square yardage for that area,
4inch + 4 inch + 1.5 inch or up to 4 inch.). Measurement shall
also include sweeping to detect metal hidden below the surface for
each 4 inch or less depth increment of pavement to be planed.
Measurement for Surface Preparation, Prelevel will be by the ton
of HMA class placed for preleveling surfaces based on the actual
quantity incorporated into the Work as determined by the Material
load tickets received and accepted by the Engineer on the day the
Material was delivered and placed.
Measurement of permanent pavement patching will be by the ton
for the HMA class specified. Measurement of temporary pavement
patch will be made by the ton for the initial placement only.
Additional temporary pavement patch required to maintain the
surface of the temporary patch level with adjacent roadway surfaces
will not be measured. An exception for measuring pavement patch for
electrical conduit construction as specified in Section 8-33 will
be based on actual measured dimensions with the width of
restoration no greater than 24 inches.
Measurement of Material Transfer Vehicle (MTV) will be made by
the ton of HMA transferred through the MTV and placed. Measurement
will not be made for Material Transfer Vehicle (MTV) for placed HMA
not transferred through the MTV.
5-04.5 PAYMENT Compensation for the cost necessary to complete
the work described in Section 5-04 will be made
at the Bid item prices Bid only for the Bid items listed or
referenced as follows: 1. Pavement, HMA (Class), per ton.
The Bid item price for Pavement, HMA (Class) shall include all
costs for the work required to furnish, haul, place and compact the
HMA mix, including tack coat, fog seal and sealing joints and meet
lines, sand for joints and meet lines, cleaning, and such other
work as may be necessary and not otherwise set forth as a separate
Bid item in the Bid Form. 2. Roadway Preparation, per linear
The Bid item price for Roadway Preparation shall include all
costs for the work required to prepare the untreated roadway,
including scarifying, blading, shaping, and compacting to remove
irregularities and secure a uniform surface except prime coat
treatment which will be paid in accordance with Section 5-02. 3.
Surface Preparation, Prelevel, per ton.
The Bid item price for Surface Preparation, Prelevel shall
include all costs for the work required to prelevel uneven or
broken treated surfaces by placing and compacting asphalt as
specified in Section 5-04.3(4)B2. 4. Surface Preparation, Plane
Bituminous Pavement, per square yard.
The Bid item price for Surface Preparation, Plane Bituminous
Pavement shall include all costs for the work required to prepare
the treated surface including sweeping for hidden metal, exposing
metal below the pavement surface where indicated on the Drawings
before planing, milling and planing and other type pavement removal
as may be necessary, removing and disposing of cuttings, extra
planing for butt joints, and feathering meet areas in preparation
for an asphalt overlay. 5. Crack Sealing, per linear foot.
The Bid item price for Crack Sealing shall include all costs for
the work required to clean and fill the cracks and joints. 6.
Pavement Patch, Temporary, per ton.
The Bid item price for Pavement Patch, Temporary shall include
all costs for the work required to install and remove the temporary
patch. The costs for additional Material required to maintain
temporary pavement patches after the initial installation shall be
at the sole expense of the Contractor. 7. Material Transfer Vehicle
(MTV), per ton. The Bid item price for Material Transfer Vehicle
(MTV) shall include all costs for the work required to place HMA
through the MTV. All cost for the MTV not included in Material
Transfer Vehicle (MTV) shall be included in other Bid items and no
separate or additional payment will be made therefore. 8. Other
Payment for Mineral Aggregate (Type) will be made in accordance
with Section 4-01.5. Payment for removal will be made in accordance
with Section 2-02.5. All costs for the rejection and disposal of
Materials held for more than 24 hours after mixing, as
specified in Section 5-04.3(8), shall be at the Contractors sole
expense and at no additional or separate cost to the Owner.
When cores are taken by the Engineer at the request of the
Contractor, the Owner shall be reimbursed for the coring expenses
as specified in Section 1-05.7.
Where samples have been taken by the Engineer from the
uncompressed asphalt concrete, new Material shall be placed and
compacted at no additional expense to the Owner.
Where the Engineer accepts area of pavement that does not meet
the smoothness requirement as specified in Section 5-04.3(12)A, the
total payment for yardage of that pavement will be reduced by
$500.00 for each and every increment of section of a single traffic
lane of 100 feet in length. Where more than 100 feet of such
pavement exists, whether in one or more lanes, payment will be
reduced as described. Payment for the last incremental section of
said pavement will be reduced by $500.00 if such last incremental
section is less than 100 feet.
Where the placement of asphalt for Portland cement concrete
overlay requires grinding to provide for the full thickness of
concrete pavement overlay, all expense for grinding shall be at the
Contractors sole expense and no separate or additional payment will
be made therefore.
Payment for backfill and compaction of the subgrade shall be
included in the Bid item price for the particular Bid item(s) of
Work necessitating such work.
Payment for subgrade preparation as required by Section
5-04.3(4)C1 will be in accordance with Section 2-06.5.
Payment for Material used for fog seal as specified in Section
5-04.3(18) will be paid as asphalt for tack coat, except no payment
will be made for sealing pavement that has been repaired as
specified in Section 5-04.3(12).
All costs for anti-stripping additive as specified in Sections
5-04.3(6) and 5-04.3(19) shall be incidental to and included in the
applicable Bid item prices and no separate or additional payment
will be made.
All costs for temporary pavement marking and removal shall be
incidental to and included in the applicable Bid item prices and no
separate or additional payment will be made therefore.
All costs to repair pavement damaged by the removal of temporary
marking tape specified in Section 5-04.3(17) shall be at the
Contractors sole expense and no additional or separate payment will
be made therefore.
All cost to repair existing pavement to remain, that is damaged
by the Contractors planing as specified in Sections 5-04.3(4)B2 and
5-04.3(4)B3, shall be at the sole expense of the Contractor and no
separate or additional payment will be made therefore.
If the Contractor requests and the Engineer approves a change in
grade of asphalt binder as specified in Section 5-04.2(1), the
Contractor accepts no change in the Bid item price, and no separate
or additional payment will be made therefore.
All cost associated with Contractor proposed and Engineer
approved use of RAP, a